- Home
- Documents
*Finite Element Approximation of Finite Deformation Dislocation 2020-04-06¢ Finite Element...*

prev

next

out of 70

View

5Download

0

Embed Size (px)

Finite Element Approximation of Finite Deformation Dislocation Mechanics

Rajat Arora∗ Xiaohan Zhang† Amit Acharya‡

Abstract

We develop and demonstrate the first general computational tool for finite deformation static and dynamic dislocation mechanics. A finite element formulation of finite de- formation (Mesoscale) Field Dislocation Mechanics theory is presented. The model is a minimal enhancement of classical crystal/J2 plasticity that fundamentally accounts for polar/excess dislocations at the mesoscale. It has the ability to compute the static and dynamic finite deformation stress fields of arbitrary (evolving) dislocation distribu- tions in finite bodies of arbitrary shape and elastic anisotropy under general boundary conditions. This capability is used to present a comparison of the static stress fields, at finite and small deformations, for screw and edge dislocations, revealing heretofore unexpected differences. The computational framework is verified against the sharply contrasting predictions of geometrically linear and nonlinear theories for the stress field of a spatially homogeneous dislocation distribution in the body, as well as against other exact results of the theory. Verification tests of the time-dependent numerics are also presented. Size effects in crystal and isotropic versions of the theory are shown to be a natural consequence of the model and are validated against available experimental data. With inertial effects incorporated, the development of an (asymmetric) propa- gating Mach cone is demonstrated in the finite deformation theory when a dislocation moves at speeds greater than the linear elastic shear wave speed of the material.

1 Introduction

Before the advent of the finite element (FE) method, solving boundary value problems of elasticity theory in any generality, especially for practical purposes of engineering design, was an essentially impossible task. That state of affairs has significantly changed today, with the approximation of solutions to complex problems of industrial design having become routine,

∗Dept. of Civil & Environmental Engineering, Carnegie Mellon University, Pittsburgh, PA, 15213. Cur- rently: R&D Engg. II, Ansys, Inc. rajat.arora9464@gmail.com. †Senior Data Scientist, Salesforce.com, Sunnyvale, CA, 94086. xiaohanzhang.cmu@gmail.com. ‡Dept. of Civil & Environmental Engineering, and Center for Nonlinear Analysis, Carnegie Mellon Uni-

versity, Pittsburgh, PA, 15213. acharyaamit@cmu.edu.

1

with even robust commercial FE software being available for such tasks. A similar situa- tion exists today in materials science related to a large class of important problems. Many materials physics problems in structural and electronic materials demand the comparison of stress and energy density fields of two (or more) specific defect distributions in an elas- tically anisotropic, possibly inhomogeneous, body of geometrically complex shape, in order to determine which may be energetically more favorable and therefore physically observable (as a first estimate). For example, a first guess at whether dislocation nucleation is possible or not in a nanostructure may be addressed by computing the total energy content of the loaded structure without defects at finite deformation, and comparing this energy content with energy content of the body containing the putative, expected defect configuration to be nucleated - the Matthews-Blakeslee critical thickness criterion for strained epitaxial het- erostructures is very much in this spirit. These are problems that involve large elastic strains, elastic anisotropy and often, inhomogeneity, and finite bodies - and, today, there exists no general purpose capability to address such questions of design (and theory), taking the bur- den of creative, ad-hoc, case-by-case approximation off of the analyst and transferring it to a robust computational capability based on fundamental principles. As part of this paper, we present such a framework. The presented development can also perform several other important tasks relevant to the materials science of hard solids (as well as soft, e.g. liquid crystal elastomers) where defects play an important role.

Conventional elasto-plastic theories model plastic flow through constituitive assumptions without explicitly recognizing dislocation motion. Owing to the lack of an inherent length scale, these theories also fail to capture any size dependence in the elasto-plastic response of (homogeneous) materials. However, it is now well-established through a vast literature, e.g. [FMAH94, LHT+12, SWBM93, EA66, MC95, SE98] that metals exhibit size effects at micron to submicron length scales. For example, there is a strong size effect in the mea- sured indentation hardness of single crystals when the indenter size is below 10 microns [MC95, SWBM93]. For a given volume fraction of elastic particles in a ductile metal, the strengthening is greater for smaller particle size [EA66, KN63]. Another example is that un- der torsional loading of copper wires, the scaled shear strength, as a function of average shear strain, has been shown to increase by a factor of around 3 as the wire diameter is reduced from 100 microns to 10 microns [FMAH94, LHT+12], with negligible size effect observed un- der tensile load. Direct support for the notion that GNDs, so-called geometrically-necessary dislocations or polar/excess dislocation density at the mesoscale, lead to enhanced hardening comes from the experiments performed in [RA70]. The prediction of size-dependent behavior requires the presence of an inherent length scale in the theory based on dimensional grounds.

Beyond hardening in the material, dislocations have also been observed to develop intri- cate microstructures under the action of their mutual interactions and applied loads such as dislocation cells [MW76, MAH79, MHS81, HH00] and labyrinths [JW84], often with dipolar dislocation walls, and mosaics [TCDH95]. The presence of such dislocation microstructures, in particular their ‘cell size’ and orientations can have a strong influence on the macroscopic response of materials [HH12, Ree06].

To our knowledge, there is no continuum formulation that takes into account the stress field of signed dislocation density and its transport at finite deformation and can predict re-

2

alistic microstructure development. Toupin’s couple-stress elasticity theory [Tou62] is com- putationally implemented within the Isogeometric Analysis method in [WRG16] to compute the stress fields of static dislocations at finite strains, representing defects by force dipole distributions. As shown there, the force-dipole representation is ‘non-local’ w.r.t repre- senting a dislocation line/loop and therefore can become onerous for computing the static field of a complex network of dislocations as well as its stress-coupled evolution. Computa- tional implementations of gradient plasticity models at finite deformation of various flavors [AB00b, APBB04, TCAS04, EBG04, KT08, MRR06, NR04, NT05, LNN19, NT19, EB17, KM19, LFB+18], including inertia [Kur19], have been developed with the goal of predicting length-scale effects, with some accounting for some version of dislocation transport; none of these models, however, can compute the stress field of a specified dislocation distribu- tion. The use of Discrete Dislocation Dynamics (DD) and Molecular Dynamics to model elastic-plastic material response and microstructure development at realistic time scales and mesoscopic length scales is currently an active area of research, as is the development of continuum scale models that can overcome the limitations of conventional theories – model- ing size effects, calculating finite deformation stress fields of signed dislocation density, and predicting (realistic) microstructure in the material. All DD models take the closed-form stress fields of individual dislocations as input. Current versions of DD accounting for some features of finite deformation have been reviewed in [AA19] - these models are not capable of computing the finite deformation stress and energy density fields of dislocation distri- butions. This paper reports the development of one such model by developing a mechanics based, novel parallel computational tool to make finite element method based computational predictions of finite deformation dislocation plasticity.

The current work presents a numerical framework based on Field Dislocation Mechanics (FDM) theory [Ach01, Ach03, Ach04], an extension of conventional plasticity that exactly accounts for the finite deformation stress fields of dislocations and their spatio-temporal evolution, for solving a large class of initial boundary value problems in finite strain dislo- cation mechanics at microscopic scales. A model for mesoscale plasticity, Mesoscale Field Dislocation Mechanics (MFDM) [AR06, Ach11], was developed from FDM by elementary averaging techniques utilized in the study of multiphase flows (see e.g. [Bab97]). This av- eraging procedure does not provide closure equations, and the resulting structure can be interpreted, for operational purposes, as the equations of FDM augmented by an extra term. This term describes the plastic strain rate due to unresolved dislocations and is phenomeno- logically specified in MFDM. Despite the phenomenology, the averaging procedure and the fine-scale theory involved impart to the coarse model a rich structure that enables a gamut of relevant predictions, with only two extra material parameters over and above conventional macroscopic continuum plasticity.

The finite-element formulation for finite deformation MFDM, presented subsequently, uses an updated Lagrangian description. The formulation generalizes the FEM implementation of small deformation